LMucko/crystallography-open-database huggingface dataset:
Crystal structure of cobalt(II) orthophosphate monohydrate, Co3 (P O4)2 H2 O
Anderson, J.; Kostiner, E.; Ruszala, F.A.; Inorganic Chemistry 15 (1976) 2744–2748; doi:

data_4343554
_publ_section_title
;
 Crystal structure of cobalt(II) orthophosphate monohydrate, Co3 (P O4)2
 H2 O
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2744
_journal_page_last               2748
_journal_volume                  15
_journal_year                    1976
_chemical_formula_sum            'Co3 H2 O9 P2'
_chemical_name_systematic        'Co3 (P O4)2 (H2 O)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.15
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.523
_cell_length_b                   7.903
_cell_length_c                   9.294
_cell_volume                     638.250
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Anderson_INOCAJ_1976_381.cif
_cod_data_source_block           H2Co3O9P2
_cod_original_cell_volume        638.2496
_cod_original_formula_sum        'H2 Co3 O9 P2'
_cod_database_code               4343554
Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1 Tin-2 Cr2 O2n-1
Andersson, S.; Jahnberg, L.; Arkiv foer Kemi 21 (1963) 413–426; doi:

data_1520779
_publ_section_title
;
 Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1
 Tin-2 Cr2 O2n-1
;
_journal_name_full               'Arkiv foer Kemi'
_journal_page_first              413
_journal_page_last               426
_journal_volume                  21
_journal_year                    1963
_chemical_formula_sum            'O9 Ti5'
_chemical_name_systematic        'Ti5 O9'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                97.6
_cell_angle_beta                 112.3
_cell_angle_gamma                108.5
_cell_formula_units_Z            2
_cell_length_a                   5.6
_cell_length_b                   7.12
_cell_length_c                   8.87
_cell_volume                     297.161
_citation_journal_id_ASTM        ARKEAD
_cod_data_source_file            Andersson_ARKEAD_1963_1374.cif
_cod_data_source_block           O9Ti5
_cod_original_cell_volume        297.1606
_cod_database_code               1520779
Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1 Tin-2 Cr2 O2n-1
Andersson, S.; Jahnberg, L.; Arkiv foer Kemi 21 (1963) 413–426; doi:

data_1520780
_publ_section_title
;
 Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1
 Tin-2 Cr2 O2n-1
;
_journal_name_full               'Arkiv foer Kemi'
_journal_page_first              413
_journal_page_last               426
_journal_volume                  21
_journal_year                    1963
_chemical_formula_sum            'O11 Ti6'
_chemical_name_systematic        'Ti6 O11'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                98.5
_cell_angle_beta                 120.8
_cell_angle_gamma                108.5
_cell_formula_units_Z            4
_cell_length_a                   5.56
_cell_length_b                   7.14
_cell_length_c                   24.04
_cell_volume                     718.779
_citation_journal_id_ASTM        ARKEAD
_cod_data_source_file            Andersson_ARKEAD_1963_1382.cif
_cod_data_source_block           O11Ti6
_cod_original_cell_volume        718.7791
_cod_database_code               1520780
Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1 Tin-2 Cr2 O2n-1
Andersson, S.; Jahnberg, L.; Arkiv foer Kemi 21 (1963) 413–426; doi:

data_1520781
_publ_section_title
;
 Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1
 Tin-2 Cr2 O2n-1
;
_journal_name_full               'Arkiv foer Kemi'
_journal_page_first              413
_journal_page_last               426
_journal_volume                  21
_journal_year                    1963
_chemical_formula_sum            'O13 Ti7'
_chemical_name_systematic        'Ti7 O13'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                98.9
_cell_angle_beta                 125.5
_cell_angle_gamma                108.5
_cell_formula_units_Z            2
_cell_length_a                   5.54
_cell_length_b                   7.13
_cell_length_c                   15.36
_cell_volume                     420.855
_citation_journal_id_ASTM        ARKEAD
_cod_data_source_file            Andersson_ARKEAD_1963_1393.cif
_cod_data_source_block           O13Ti7
_cod_original_cell_volume        420.8545
_cod_database_code               1520781
Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1 Tin-2 Cr2 O2n-1
Andersson, S.; Jahnberg, L.; Arkiv foer Kemi 21 (1963) 413–426; doi:

data_1520782
_publ_section_title
;
 Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1
 Tin-2 Cr2 O2n-1
;
_journal_name_full               'Arkiv foer Kemi'
_journal_page_first              413
_journal_page_last               426
_journal_volume                  21
_journal_year                    1963
_chemical_formula_sum            'O15 Ti8'
_chemical_name_systematic        'Ti8 O15'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                97.2
_cell_angle_beta                 128.8
_cell_angle_gamma                109.6
_cell_formula_units_Z            4
_cell_length_a                   5.57
_cell_length_b                   7.1
_cell_length_c                   37.46
_cell_volume                     967.412
_citation_journal_id_ASTM        ARKEAD
_cod_data_source_file            Andersson_ARKEAD_1963_1401.cif
_cod_data_source_block           O15Ti8
_cod_original_cell_volume        967.4123
_cod_database_code               1520782
Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1 Tin-2 Cr2 O2n-1
Andersson, S.; Jahnberg, L.; Arkiv foer Kemi 21 (1963) 413–426; doi:

data_1520783
_publ_section_title
;
 Crystal structure studies on the homologous series Tin O2n-1 Vn O2n-1
 Tin-2 Cr2 O2n-1
;
_journal_name_full               'Arkiv foer Kemi'
_journal_page_first              413
_journal_page_last               426
_journal_volume                  21
_journal_year                    1963
_chemical_formula_sum            'O17 Ti9'
_chemical_name_systematic        'Ti9 O17'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                97.1
_cell_angle_beta                 131
_cell_angle_gamma                109.8
_cell_formula_units_Z            2
_cell_length_a                   5.57
_cell_length_b                   7.1
_cell_length_c                   22.15
_cell_volume                     543.261
_citation_journal_id_ASTM        ARKEAD
_cod_data_source_file            Andersson_ARKEAD_1963_1408.cif
_cod_data_source_block           O17Ti9
_cod_database_code               1520783
Neutron powder diffraction investigations of Nb3 (Al0.84 Nb0.16) and Nb3 (Al0.84 Nb0.16) (2)H2.52
Andersson, Y.; Rundqvist, S.; Nolang, B.; Larsson, T.; Journal of Alloys Compd. 306 (2000) 193–196; doi:

data_1520784
_publ_section_title
;
 Neutron powder diffraction investigations of Nb3 (Al0.84 Nb0.16) and Nb3
 (Al0.84 Nb0.16) (2)H2.52
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              193
_journal_page_last               196
_journal_volume                  306
_journal_year                    2000
_chemical_formula_sum            'Al0.84 D2.52 Nb3.16'
_chemical_name_systematic        'Nb3 (Al0.84 Nb0.16) D2.52'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.3627
_cell_length_b                   5.3627
_cell_length_c                   5.3627
_cell_volume                     154.223
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Andersson_JALCEU_2000_1369.cif
_cod_data_source_block           D2.52Al0.84Nb3.16
_cod_original_cell_volume        154.2235
_cod_original_formula_sum        'D2.52 Al0.84 Nb3.16'
_cod_database_code               1520784
Neutron diffraction study of the magnetic and structure properties of Co2.50 Sb0.50 O4 spinel
Antic, B.; Tellgren, R.; Rodic, D.; Rundlof, H.; Journal of Magnetism and Magnetic Materials 219 (2000) 41–44; doi:

data_1520785
_publ_section_title
;
 Neutron diffraction study of the magnetic and structure properties of
 Co2.50 Sb0.50 O4 spinel
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              41
_journal_page_last               44
_journal_volume                  219
_journal_year                    2000
_chemical_formula_sum            'Co2.5 O4 Sb0.5'
_chemical_name_systematic        'Co (Co1.5 Sb0.5) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.469
_cell_length_b                   8.469
_cell_length_c                   8.469
_cell_volume                     607.430
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Antic_JMMMDC_2000_1574.cif
_cod_data_source_block           Co2.5O4Sb0.5
_cod_original_cell_volume        607.4302
_cod_database_code               1520785
Ludwigite from central Sweden: new data and crystal structure refinement
Appel, P.W.U.; Brigatti, M.F.; Mineralogical Magazine (1969-) 63 (1999) 511–518; doi:

data_1520786
_publ_section_title
;
 Ludwigite from central Sweden: new data and crystal structure refinement
;
_journal_name_full               'Mineralogical Magazine (1969-)'
_journal_page_first              511
_journal_page_last               518
_journal_volume                  63
_journal_year                    1999
_chemical_formula_sum            'Al0.093 B Fe0.967 Mg1.93 O5'
_chemical_name_systematic        '(Mg1.93 Fe0.967 Al0.093) O2 (B O3)'
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.254
_cell_length_b                   12.287
_cell_length_c                   3.004
_cell_volume                     341.567
_citation_journal_id_ASTM        MNLMBB
_cod_data_source_file            Appel_MNLMBB_1999_487.cif
_cod_data_source_block           Al0.093B1Fe0.967Mg1.93O5
_cod_original_cell_volume        341.5665
_cod_original_formula_sum        'Al0.093 B1 Fe0.967 Mg1.93 O5'
_cod_database_code               1520786
Lithium nickelate electrodes with enhanced high-temperature performance and thermal stability
Arai, H.; Tsuda, M.; Sakurai, Y.; Journal of Power Sources 90 (2000) 76–81; doi:

data_1520787
_publ_section_title
;
 Lithium nickelate electrodes with enhanced high-temperature performance
 and thermal stability
;
_journal_name_full               'Journal of Power Sources'
_journal_page_first              76
_journal_page_last               81
_journal_volume                  90
_journal_year                    2000
_chemical_formula_sum            'Li1.01 Mn0.1 Ni0.89 O2'
_chemical_name_systematic        '(Li0.97 Ni0.03) (Li0.04 Ni0.86 Mn0.1) O2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   2.8709
_cell_length_b                   2.8709
_cell_length_c                   14.179
_cell_volume                     101.207
_citation_journal_id_ASTM        JPSODZ
_cod_data_source_file            Arai_JPSODZ_2000_1636.cif
_cod_data_source_block           Li1.01Mn0.1Ni0.89O2
_cod_original_cell_volume        101.2074
_cod_database_code               1520787
Lithium nickelate electrodes with enhanced high-temperature performance and thermal stability
Arai, H.; Tsuda, M.; Sakurai, Y.; Journal of Power Sources 90 (2000) 76–81; doi:

data_1520788
_publ_section_title
;
 Lithium nickelate electrodes with enhanced high-temperature performance
 and thermal stability
;
_journal_name_full               'Journal of Power Sources'
_journal_page_first              76
_journal_page_last               81
_journal_volume                  90
_journal_year                    2000
_chemical_formula_sum            'Li1.02 Ni0.88 O2 Ti0.1'
_chemical_name_systematic        '(Li0.98 Ni0.02) (Li0.04 Ni0.86 Ti0.1) O2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   2.8766
_cell_length_b                   2.8766
_cell_length_c                   14.215
_cell_volume                     101.868
_citation_journal_id_ASTM        JPSODZ
_cod_data_source_file            Arai_JPSODZ_2000_1637.cif
_cod_data_source_block           Li1.02Ni0.88O2Ti0.1
_cod_original_cell_volume        101.8677
_cod_database_code               1520788
Lithium nickelate electrodes with enhanced high-temperature performance and thermal stability
Arai, H.; Tsuda, M.; Sakurai, Y.; Journal of Power Sources 90 (2000) 76–81; doi:

data_1520789
_publ_section_title
;
 Lithium nickelate electrodes with enhanced high-temperature performance
 and thermal stability
;
_journal_name_full               'Journal of Power Sources'
_journal_page_first              76
_journal_page_last               81
_journal_volume                  90
_journal_year                    2000
_chemical_formula_sum            'Co0.1 Li1.03 Mn0.1 Ni0.77 O2'
_chemical_name_systematic
'(Li0.98 Ni0.02) (Li0.05 Ni0.75 Co0.1 Mn0.1) O2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   2.8645
_cell_length_b                   2.8645
_cell_length_c                   14.161
_cell_volume                     100.629
_citation_journal_id_ASTM        JPSODZ
_cod_data_source_file            Arai_JPSODZ_2000_1638.cif
_cod_data_source_block           Co0.1Li1.03Mn0.1Ni0.77O2
_cod_original_cell_volume        100.6288
_cod_database_code               1520789
Lithium nickelate electrodes with enhanced high-temperature performance and thermal stability
Arai, H.; Sakurai, Y.; Tsuda, M.; Journal of Power Sources 90 (2000) 76–81; doi:

data_1520790
_publ_section_title
;
 Lithium nickelate electrodes with enhanced high-temperature performance
 and thermal stability
;
_journal_name_full               'Journal of Power Sources'
_journal_page_first              76
_journal_page_last               81
_journal_volume                  90
_journal_year                    2000
_chemical_formula_sum            'Co0.1 Li1.03 Ni0.77 O2 Ti0.1'
_chemical_name_systematic
'(Li0.98 Ni0.02) (Li0.05 Ni0.75 Co0.1 Ti0.1) O2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   2.8753
_cell_length_b                   2.8753
_cell_length_c                   14.215
_cell_volume                     101.776
_citation_journal_id_ASTM        JPSODZ
_cod_data_source_file            Arai_JPSODZ_2000_1639.cif
_cod_data_source_block           Co0.1Li1.03Ni0.77O2Ti0.1
_cod_original_cell_volume        101.7756
_cod_database_code               1520790
K Nb4 O5 F and Nb O2 crystal structures. Structural aspect of chemical decomposition of K2-x Nb4 O3 (O, F)3 F in the melt of sodium and potassium chlorides
Arakcheeva, A.V.; Shamrai, V.F.; Grinevich, V.V.; Meyer, M.; Chapuis, G.; Kristallografiya 44 (1999) 6–11; doi:

data_1520791
_publ_section_title
;
 K Nb4 O5 F and Nb O2 crystal structures. Structural aspect of chemical
 decomposition of K2-x Nb4 O3 (O, F)3 F in the melt of sodium and
 potassium chlorides
;
_journal_name_full               Kristallografiya
_journal_page_first              6
_journal_page_last               11
_journal_volume                  44
_journal_year                    1999
_chemical_formula_sum            'Nb O2'
_space_group_IT_number           88
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            32
_cell_length_a                   13.698
_cell_length_b                   13.698
_cell_length_c                   5.976
_cell_volume                     1121.308
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1999_440.cif
_cod_data_source_block           Nb1O2
_cod_original_formula_sum        'Nb1 O2'
_cod_database_code               1520791
K Nb4 O5 F and Nb O2 crystal structures. Structural aspect of chemical decomposition of K2-x Nb4 O3 (O, F)3 F in the melt of sodium and potassium chlorides
Arakcheeva, A.V.; Grinevich, V.V.; Chapuis, G.; Shamrai, V.F.; Meyer, M.; Kristallografiya 44 (1999) 6–11; doi:

data_1520792
_publ_section_title
;
 K Nb4 O5 F and Nb O2 crystal structures. Structural aspect of chemical
 decomposition of K2-x Nb4 O3 (O, F)3 F in the melt of sodium and
 potassium chlorides
;
_journal_name_full               Kristallografiya
_journal_page_first              6
_journal_page_last               11
_journal_volume                  44
_journal_year                    1999
_chemical_formula_sum            'F K Nb4 O5'
_chemical_name_systematic        'K Nb4 O5 F'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.155
_cell_length_b                   4.155
_cell_length_c                   8.377
_cell_volume                     144.621
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1999_441.cif
_cod_data_source_block           F1K1Nb4O5
_cod_original_cell_volume        144.6207
_cod_original_formula_sum        'F1 K1 Nb4 O5'
_cod_database_code               1520792
Perovskite-like modification of Cs3 Sb2 I9 as a member of the OD family A3 B2 X9
Arakcheeva, A.V.; Novikova, M.S.; Lubman, G.U.; Zaitsev, A.I.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 40 (1999) 705–715; doi:

data_1520793
_publ_section_title
;
 Perovskite-like modification of Cs3 Sb2 I9 as a member of the OD family
 A3 B2 X9
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              705
_journal_page_last               715
_journal_volume                  40
_journal_year                    1999
_chemical_formula_sum            'Cs3 I9 Sb2'
_chemical_name_systematic        'Cs3 (Sb2 I9)'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.435
_cell_length_b                   8.435
_cell_length_c                   10.39
_cell_volume                     640.201
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Arakcheeva_ZSTKAI_1999_933.cif
_cod_data_source_block           Cs3I9Sb2
_cod_original_cell_volume        640.2011
_cod_database_code               1520793
On the space group of garronite
Artioli, G.; Marchi, M.; Powder Diffraction 14 (1999) 190–194; doi:

data_1520794
_publ_section_title
;
 On the space group of garronite
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              190
_journal_page_last               194
_journal_volume                  14
_journal_year                    1999
_chemical_formula_sum            'Al5.84 Ca2.89 H32.64 O48.32 Si10.16'
_chemical_name_systematic        'Ca2.89 (Al5.84 Si10.16 O32) (H2 O)16.32'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-I 2ya'
_symmetry_space_group_name_H-M   'I 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.113
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.8799
_cell_length_b                   10.2801
_cell_length_c                   9.8764
_cell_volume                     1003.108
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Artioli_PODIE2_1999_684.cif
_cod_data_source_block           H32.64Al5.84Ca2.89O48.32Si10.16
_cod_original_sg_symbol_Hall     '-C 2yc (x+z,y,-x)'
_cod_original_formula_sum        'H32.64 Al5.84 Ca2.89 O48.32 Si10.16'
_cod_database_code               1520794
Distribution of metal ions and magnetic susceptibility in Cu Ga Mn O4 spinel
Asbrink, S.; Waskowska, A.; Talik, E.; Journal of Physics and Chemistry of Solids 60 (1999) 573–577; doi:

data_1520795
_publ_section_title
;
 Distribution of metal ions and magnetic susceptibility in Cu Ga Mn O4
 spinel
;
_journal_name_full               'Journal of Physics and Chemistry of Solids'
_journal_page_first              573
_journal_page_last               577
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Cu Ga1.01 Mn0.99 O4'
_chemical_name_systematic
'(Cu0.7 Mn0.27 Ga0.03) (Cu0.15 Mn0.36 Ga0.49)2 O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.387
_cell_length_b                   8.387
_cell_length_c                   8.387
_cell_volume                     589.956
_citation_journal_id_ASTM        JPCSAW
_cod_data_source_file            Asbrink_JPCSAW_1999_228.cif
_cod_data_source_block           Cu1Ga1.01Mn0.99O4
_cod_original_cell_volume        589.9564
_cod_original_formula_sum        'Cu1 Ga1.01 Mn0.99 O4'
_cod_database_code               1520795